Through a facile solvothermal procedure, a CdS/WOx nanocomposite has been synthesised which exhibits photocapacitive behaviour under white light illumination at a radiant flux density of 99.3 mW cm−2. Photoelectrochemical experiments were undertaken to examine the self-charging properties of the material and to develop an understanding of the underlying electronic band structure responsible for the phenomenon. By employing XPS, UPS and UV-Vis diffuse reflectance spectroscopy for further characterisation, the ability of the composite to generate current following the removal of incident light was related to the trapping of photoexcited electrons by the WOx component. The presence of WOx yielded an order of magnitude increase in the transient photocurrent response relative to CdS alone, an effect attributed to the suppression of electron-hole recombination in CdS due to hole transfer across the CdS/WOx interface. Moreover, current discharge from the material persisted for more than twenty minutes after final illumination, an order of magnitude improvement over many existing binary composites. As a seminal investigation into the photocapacitive characteristics of CdS/WOx composites, the work offers insight into how the constituent materials might be utilised as part of a future self-charging solar device.
As a consequence of the global shift towards renewable sources of energy, the development of energy storage technologies has grown increasingly important. Indeed, if the world is to substitute traditional fossil fuels for variable and unpredictable alternatives such as solar or wind power, energy from these sources must be stored during periods of surplus supply for times of excess demand. To this end, consumers are beginning to explore the benefits of household battery systems as a storage medium for solar energy1,2,3, and there are also multiple larger-scale energy storage projects currently planned or underway across the globe4. An alternative solution is the use of electrolysers to store surplus energy in the form of hydrogen5,6,7, a commodity which may be used to generate electricity directly through use of fuel cells8,9 or otherwise combusted in the manner of a conventional fuel gas10.
Despite the practicability of existing storage technologies, their widespread implementation is inhibited by factors such as the financial cost of necessary infrastructure11,12,13,14 and their unsuitability in size-limited applications15,16. The prospect of in situ energy storage is therefore an attractive one: by simultaneously generating electrical power and storing surplus energy within a single device, the need for an external storage medium is bypassed. The potential of such an approach has been most notably showcased by photocapacitive “self-charging” solar cells15,16,17,18,19,20,21,22,23,24,25,26,27,28,29, which serve as a source of electrical power under solar illumination whilst simultaneously retaining a proportion of the incident energy in the form of a stored electrical charge. The earliest example of a such a device incorporated titanium dioxide as a UV-absorbing component and a supercapacitor comprised of layers of activated carbon with a porous separator, all integrated into a single monolithic device24. The success of a self-charging solar cell depends not only on the physical and chemical properties of its photoactive and supercapacitive components, but also the intimacy of the electronic junction between them.
In the present investigation, the photocapacitive behaviour of a nanocomposite of cadmium sulphide, CdS, and tungsten(VI) sub-oxide, WOx, is explored under white light illumination at a power density of approximately one Sun. The constituents of this composite, which shall be henceforth referred to as CdS/WOx, were selected for their respective photoabsorbance and surface-reactivity characteristics; CdS, for instance, has a typical photonic band-gap of 2.4 eV30,31,32,33, and is consequently a proficient absorber of visible light. Moreover, the electron mobility in CdS is typically in the range 1–10 cm2 V s−1, similar to reported values for TiO234,35,36,37,38. A primary drawback of CdS, however, is its susceptibility to photocorrosion, although the phenomenon may be suppressed through the efficient scavenging of photoinduced holes39,40,41,42,43,44. By incorporating the material into a composite of strategically-selected constituents, it is therefore possible to improve the stability of CdS whilst preserving its desirable properties.
As the second component of the composite, WOx typically provides a high surface area due to the propensity of the material to form crystalline nanostructures45, and the intrinsic oxygen vacancies function as both reactive surface sites46,47,48,49 and electron donor states50,51,52, as well as allowing the material to operate as an effective electron sink53,54,55,56,57,58. By employing a solvothermal approach used previously by the present researchers59, WOx nanostructures may be grown heterogeneously from the surface of pre-synthesised particles to promote an intimate junction between the constituent materials. Herein, the CdS/WOx nanostructures so-formed are tested using a three-electrode photoelectrochemical setup to verify their applicability to photocapacitive applications, exploring the electrical behaviour during and after white light exposure and the stability of the response following prolonged illumination. The study aims not to demonstrate the function of a completed self-charging solar cell, but rather it serves to identify the physical interplay between CdS and WOx and to elucidate how a workable self-charging CdS/WOx device might be realised.
As shown by the SEM image in Fig. 1a, the solvothermal synthesis of CdS yielded nanoparticles with a typical diameter of less than 200 nm, although it was difficult to acquire precise size estimates due to particle aggregation. Subsequent heterogeneous growth of WOx sub-oxides on the CdS surface yielded the morphology depicted in Fig. 1b; the WOx nanowires shown in this SEM image are characteristic of those grown solvothermally in the formation of other composites59,60,61,62, most notably the Ta3N5/WOx sample synthesised via a near-identical protocol in a previous report by the present group59. Making use of this similarity between the CdS/WOx and Ta3N5/WOx composites, the latter is employed as a reference sample in the present study to facilitate understanding of how photoelectrochemical measurements from CdS/WOx are related to electronic interactions between the two components.
A key consideration for an electrode material is its crystallinity, which may be characterised through use of XRD. Annotated on the diffractograms of CdS (Fig. 2a) and CdS/WOx (Fig. 2b) are the peaks corresponding to the hexagonal wurtzite α-CdS phase, otherwise known as greenockite (with peaks identified by black circles)63,64,65,66,67,68,69,70,71, cubic sphalerite β-CdS, or hawleyite (identified by grey circles)66,67,68,69,70,71, and monoclinic W18O49 (marked by white circles)72,73,74, as indexed by JCPDS reference cards 41–1049, 10‐0454 and 71–2450, respectively. Due to overlaps between the diffractogram peaks of α-CdS and β-CdS, it is difficult to discern the relative composition of the two phases; the high relative intensity of the peak at 26.5°, however, implies that both phases were present in the samples. The diffuse background in each diffractogram is indicative of disorder within the material associated with lattice defects; this feature is most clearly apparent in the case of CdS/WOx, and the diffuse scattering is possibly attributable to oxygen vacancies within the WOx component75.
The surface chemical composition of each sample was investigated using XPS. The survey spectrum of CdS (Fig. 3a) is accompanied by higher-resolution scans of the Cd 3d (b), S 2p (c), O 1 s (d) and C 1 s (e) photoelectron peaks, as well as the Cd MNN Auger peak (f), while the survey spectrum of CdS/WOx (Fig. 4a) is displayed alongside scans of the Cd 3d (b), S 2p (c), O 1 s (d), C 1 s (e) and W 4f (f) photoelectron peaks. The measured data in each case is represented by circular black markers connected by straight lines, with dashed black lines used for both the Shirley background function and the fitted envelope obtained from the sum of the coloured Gaussian-Lorentzian fitting components; for ease of interpretation, components corresponding to the same peak doublet are plotted in the same colour, while alternative colours are used to represent different chemical environments.
In the case of the CdS sample, it is clear that both the Cd 3d and S 2p peaks are well-fitted by a single pair of doublet components with spin-orbit separation values of 6.74 eV76,77 and 1.18 eV78,79, respectively, and the form of the Cd MNN Auger signal is characteristic of CdS80,81. The purity of the CdS surface is belied, however, by the relative areas of the Cd 3d and S 2p peaks: the measured Cd/S atomic ratio of 1.42 is significantly higher than the expected value of unity, indicating the presence of other Cd-containing compounds. Indeed, the form of the O 1 s peak provides further evidence of these surface species: the component centred at 531.7 eV is consistent with compounds such as Cd(OH)2 or CdCO366,82,83,84,85,86,87, while the adjacent contribution at 533.0 eV has previously been attributed to OH− ions intercalated within the CdS lattice86. The final component, centred at a binding energy of 533.9 eV, is typically associated with adsorbed water66,85,86. It should be noted that adventitious organic species likely also contribute to the O 1 s spectrum, particularly the component at 533.0 eV88,89, and are also responsible for the sizeable C 1 s peak; this signal may be deconvoluted into a principal component at 284.8 eV, which is associated with C atoms contained within an aliphatic hydrocarbon chain, and secondary components at 286.6 eV and 288.5 eV, corresponding to C-O and O-C=O groups, respectively89. Ignoring the adventitious organic layer, XPS deconvolution yields a tentative estimate of surface composition: assuming that the Gaussian-Lorentzian components have been accurately designated, CdS comprised approximately 70.3% of the surface layer, with other compounds such as Cd(OH)2 accounting for the remainder. Nevertheless, EDX measurements from the CdS sample, which are displayed in Fig. S1a of the Supplementary Information alongside the estimated elemental composition in Supplementary Table S1, show that the O/C atomic ratio is consistent with the corresponding value from the underlying carbon tab, while the Cd/S atomic ratio has an estimated value of 1.04; these results suggest that whilst Cd-containing contaminants were present at the surface of each nanoparticle, the bulk consisted predominantly of CdS.
A similar analysis may be applied to CdS/WOx. The appearance of significant Cd 3d and S 2p peaks in Fig. 4 suggests that CdS was present at the composite surface: comparison of the W 4f and Cd 3d signals reveals a Cd/W atomic ratio of 0.58, implying that a high proportion of the CdS surface was exposed to the aqueous electrolyte during photoelectrochemical testing. Since the Cd/S atomic ratio from the CdS/WOx spectra has a value of 1.40, one may further infer that the CdS surface remained unaffected by the formation of WOx; indeed, EDX measurements from the CdS/WOx sample, shown in Fig. S1b of the Supplementary Information, provide support for this suggestion, as the measured elemental composition, detailed in Supplementary Table S1, reveals a bulk Cd/S atomic ratio estimate of 1.06, which is consistent with the corresponding value for CdS. One should note from the EDX spectrum that there is a greater abundance of O within the CdS/WOx sample than anticipated from WOx alone, with the surplus accounting for over half of the overall O content; since it is not possible to reconcile this result with the underlying carbon tab, which was shown to contain O at a concentration of approximately 7 at%, it is likely that preparation of the composite resulted in residual organic compounds that were not removed during subsequent centrifugation steps.
Despite the likelihood that Cd(OH)2 and other possible Cd-containing species contributed to the O 1 s peak of the CdS/WOx XPS spectrum, it should be recognised that the absolute area of the peak is 5.3 times greater than the O 1 s signal of CdS, while the Cd 3d peak of Cd/WOx is smaller than the corresponding peak of CdS by a factor of 3.0. One may therefore deduce that within the CdS/WOx sample, O 1 s contributions from the CdS surface accounted for roughly one-sixteenth of the total, and hence it is reasonable to neglect them during deconvolution of the O 1 s spectrum. The O 1 s component centred at 530.6 eV may be attributed to O atoms within the WOx lattice, while the component at 531.9 eV corresponds to O atoms at the surface of the WOx lattice and the highest energy contribution, at 533.1 eV, is again typically associated with surface species such as adsorbed water90,91,92,93,94,95,96. The small component centred at 528.5 eV cannot be reconciled with WOx, but it is consistent with CdO66,83,84,85,86; no such component was observed in the O 1 s signal of CdS, suggesting that Cd(OH)2 or other Cd-containing compounds at the CdS surface were converted to CdO during formation of the composite.
Due to partial reduction of the W6+ ions as WOx was formed, lower oxidation states of W must be considered during deconvolution of the W 4f signal. Assigning a doublet to each chemical environment, and constraining the spin-orbit separation to 2.17 eV97 in each case, the signal is well-represented by two pairs of components, with a small additional singlet at higher binding energy identified as the W 5p3/2 peak95,96. The primary contributor to the W 4f spectrum is the W6+ doublet, within which the 4f7/2 state is situated at a binding energy of 36.0 eV, while the remainder of the signal is accounted for by the W5+ doublet, which has its 4f7/2 state centred at 34.5 eV90,91,92,93,94,95,96; these component positions are in close agreement with the corresponding values of the Ta3N5/WOx composite characterised previously59, which is employed herein as a reference material. By comparing the combined areas of the W6+ and W5+ doublets to the WOx components of the O 1 s signal, one obtains a W/O atomic ratio estimate of 2.75, in close agreement with the value of 2.72 that is consistent with the formula W18O49.
It is evident from Fig. 4b,c that the positions of the Cd 3d and S 2p peaks of CdS/WOx are offset by approximately 0.5 eV with respect to their CdS counterparts in Fig. 3b,c. One should note that the spectra of both samples have been corrected by referencing the C 1 s peak to its accepted value of 284.8 eV; it is probable, therefore, that the systematic disparity in the Cd 3d and S 2p peak positions is indicative of differential charging between the CdS and WOx components of the composite, which in turn suggests that there was a significant potential barrier between the two phases at the sample surface. Indeed, the same potential offset is visible in XPS valence band measurements depicted for CdS and CdS/WOx in Fig. 5a,b, respectively: through linear extrapolation of the valence band edge to an analogous fit of the baseline data98,99,100, the valence band maximum of the CdS sample, EVB(CdS), is estimated as 1.8 eV relative to the Fermi level of the instrument (which is calibrated to 0 eV), compared to 2.3 eV in the case of CdS/WOx. It has been noted by other researchers that within a composite of photoactive and charge-trapping components, such a Schottky barrier at the inter-component interface may assist with the effective trapping of photoexcited electrons and thereby promote electron-hole separation101, in turn increasing the average lifetime of these photogenerated charges.
The appearance of electronic states close to the Fermi level in Fig. 5b is a common occurrence in WOx sub-oxides102,103,104, and the feature is indicative of populated conduction band states and associated degenerate semiconductor behaviour. By applying a linear fit to the edge of the sub-band feature, the position of the conduction band minimum of WOx, ECB(WOx), may be estimated relative to the Fermi level of the instrument; assuming that the estimate of EVB(CdS) from Fig. 5b is offset by 0.5 eV due to differential charging with respect to the WOx component, the measurements are consistent with a difference of approximately 0.4 eV between EVB(CdS) and ECB(WOx) if electronic equilibrium were to exist between the components. From these relative band edge positions one may infer that electron-hole recombination between the conduction band of WOx and valence band of CdS was thermodynamically feasible; this process of interfacial electron-hole recombination acts to suppress alternative recombination of photoexcited electrons within the photoactive phase, thereby increasing the mean lifetime of such electrons and promoting photocurrent105,106. It should be recognised that since the potential offset between CdS and WOx resulted in an increased difference between EVB(CdS) and ECB(WOx) relative to the case of electronic equilibrium between the components, the effect conceivably facilitated the process of electron-hole recombination across the inter-component interface.
The valence band maximum at the surface of each sample was further investigated using UPS; spectra from the argon-cleaned CdS and CdS/WOx samples are shown in Fig. 5c,d, respectively. By employing a protocol described elsewhere59, as detailed by Fig. S2 of the Supplementary Information and the accompanying discussion, EVB may be determined in each case from the energy difference between the secondary electron onset, Ek,SEO, and the cut-off at the valence band edge, Ek,VB: subtraction of Ek,VB-Ek,SEO from the photon energy, hν, yields an absolute value for EVB relative to the vacuum level, Evac. One should note that whilst UPS is a highly surface-sensitive technique, the obtained Ek,VB-EK,SEO estimates are typically representative of bulk values in non-degenerate semiconductors because the edges of the conduction and valence bands are fixed with respect to Evac, provided that the Fermi level is not pinned by surface states107,108,109,110,111. Previous research suggests that CdS may be assumed to satisfy this condition111,112,113,114, whereas the aforementioned bulk degeneracy of WOx is inconsistent with the standard Schottky-Mott model of band-bending; nevertheless, the occupation of conduction band states in degenerate systems precludes the formation of a space-charge region109, allowing surface band-bending to be discounted.
Based on the measurements in Fig. 5c, EVB(CdS) is estimated as 6.6 eV relative to vacuum, while Fig. 5d yields a corresponding estimate of 8.2 eV for the valence band maximum of the CdS/WOx composite. Despite the appearance of signals from both CdS and WOx in the XPS spectrum of CdS/WOx, it is instructive to note that the Ek,VB and Ek,SEO values from Fig. 5d are similar to corresponding estimates for Ta3N5/WOx and WOx obtained in a previous report;59 this similarity indicates that the EVB estimate from Fig. 5d is in turn a close approximation of the valence band maximum in WOx, and the value shall therefore be henceforth denoted EVB(WOx).
To determine the photonic band-gap of each sample, UV-Vis diffuse reflectance measurements are next addressed. The diffuse reflectance, R, of each sample, is plotted as a function of incident wavelength in Fig. 6a; by calculating the Kubelka-Munk function33,115, F(R), as a function of photon energy, hν, Tauc plots have been constructed from these measurements, as shown in Fig. 6b. Within each Tauc plot, a Matlab program was used to construct a linear fit through the points of steepest gradient, the x-intercept of which provides an estimate of the photonic band-gap; the plots of CdS and CdS/WOx yield comparable values of 2.26 eV and 2.25 eV, respectively, which are consistent with CdS band-gap estimates quoted elsewhere in the literature55,66,71,105,116,117,118. Recalling the value of EVB(CdS) from Fig. 5c, the conduction band minimum of CdS, ECB(CdS), is thus estimated as 4.3 eV relative to Evac. As ECB(WOx) cannot be estimated relative to Evac from the present results, a difference of 1.6 eV between ECB(WOx) and EVB(WOx) is to be assumed in accordance with previous work59.
By combining the values of ECB(CdS) and ECB(WOx) with the aforementioned estimates obtained from Fig. 5, one may construct a rudimentary schematic of the band positions in CdS/WOx, as illustrated in Fig. 7. One should acknowledge that whilst the values of EVB and ECB relative to Evac are generally applicable, the Fermi level positions of CdS and WOx, denoted EF(CdS) and EF(WOx), respectively, are dependent on the environment in which the composite is placed. Nevertheless, the EF estimates derived from XPS may be used to provide insight into the relative positions of the energy band edges, and for this reason a difference of 0.5 V between EF(CdS) and EF(WOx) has been assumed in the diagram, in accordance with the measured potential offset between the two components in Figs 4, 5. As the plotted values of EF(CdS) and EF(WOx) are not representative of the composite in the presence of electrolyte, the case of electronic equilibrium between the constituents shall also be addressed.
According to the estimated band positions in Fig. 7, the conduction band edge of CdS was situated approximately 1.4 eV above the minimum of the WOx conduction band, while this difference increases to 1.9 eV if one instead imposes the condition of electronic equilibrium between the components. In both scenarios, therefore, the transfer of photoexcited electrons from CdS to WOx was thermodynamically viable, permitting the accumulation of photogenerated charge at trap sites in the WOx phase. Also shown in Fig. 7 is the possible recombination of electrons from the conduction band of WOx with photoinduced holes in the valence band of CdS, thereby suppressing their recombination with photoexcited electrons; following their promotion to the conduction band of CdS, these electrons were able to either contribute to photocurrent or migrate to WOx and occupy trap sites present therein.
Placing the sample electrodes in a three-electrode configuration with an Ag/AgCl (3.0 M) reference electrode and platinum counter electrode, the transient photocurrent response of each was tested at an applied potential of 0 V in aqueous Na2SO4 electrolyte (0.5 M) under white light illumination of radiant flux density 99.3 mW cm−2; the form of the LED source spectrum is provided in Fig. S3a of the Supplementary Information, alongside details regarding calculation of the radiant flux density. In the case of CdS, for which the photocurrent behaviour at 0 V versus Ag/AgCl (3.0 M) is displayed in Fig. 8a, an instantaneous anodic response was observed upon turn-on of the LED source, followed by near-instant relaxation to zero current when illumination was removed. As shown by Fig. 8b, analogous testing of the CdS/WOx sample yielded an initial enhancement of the peak photocurrent with respect to CdS, while capacitive charging and discharging of the electrode occurred during cycling of the LED illumination. It is additionally apparent, however, that photocurrent from the CdS/WOx sample deteriorated more rapidly than in the case of CdS, exhibiting an exponential decay over the course of the experiment.
The stability of each sample may be addressed by considering its surface reactions with species present in the electrolyte. Diminishing photocurrent has been witnessed elsewhere for CdS electrodes in aqueous Na2SO4119,120, and the phenomenon is associated with the aforementioned photocorrosion of CdS by photoinduced holes due to an insufficient rate of hole-scavenging by reducing species; this effect is further evidenced by transient spikes at the start and end of each photocurrent pulse, which are characteristic of surface charge accumulation121,122,123. Degradation of the CdS sample is therefore attributable to the choice of electrolyte, and in particular the absence of effective hole-scavengers: SO42− anions are not readily oxidised on CdS surfaces due to the high reduction potentials of the SO4−˙/SO42− and S2O82−/SO42− redox couples124,125, and hole-removal was therefore dependent on the slow oxidation of water molecules126. Conversely, valence holes in WO3 and WOx sub-oxides are typically at sufficiently high potential to instigate oxidation of SO42− anions;127,128,129 the diminishing photocurrent response in Fig. 8b may be instead attributed to deactivation of the WOx component by peroxide species formed as a product of water oxidation at the catalyst surface130,131,132.
Of further interest in Fig. 8b is the magnitude of the photocurrent at the onset of illumination: prior to the aforementioned decay, the CdS/WOx system yielded an order of magnitude increase in photocurrent relative to CdS alone. The mechanism responsible for this enhancement may be explored by addressing the corresponding photoelectrochemical behaviours of the Ta3N5, Ta3N5/WOx and WOx reference samples; these measurements are displayed in Fig. S4 of the Supplementary Information. While the Ta3N5 electrode generated a transient cathodic response at the onset of illumination, Ta3N5/WOx correspondingly produced an almost indiscernible cathodic photocurrent and WOx alone exhibited negligible photoactivity; these measurements indicate that observed differences between the CdS and CdS/WOx responses cannot be ascribed to WOx in isolation, and are instead indicative of an electronic interaction between the CdS and WOx phases.
In addition to the enhancement of the photocurrent response, evidence of charge transfer between the components of CdS/WOx is provided by the pronounced capacitive charge/discharge behaviour of the composite: following the photogeneration of electron-hole pairs in CdS, the slow recombination rate upon turn-off of the light source may be attributed to an accumulation of trapped electrons in WOx133,134. At the onset of illumination, the WOx component similarly acted to retard the establishment of a stable photocurrent by extracting photoexcited electrons from CdS. Indeed, the effects of electron-trapping are further evident in open-circuit potential measurements from the CdS and CdS/WOx samples, as shown in Fig. 8c,d, respectively: of the two samples, equilibrium potential was established and removed more slowly in the case of CdS/WOx, once again demonstrating the superior charge capacity of the composite. As in the case of photocurrent, the open-circuit potential of CdS/WOx was found to diminish over the period of illumination, indicating once more that the material surface was affected detrimentally by species present in the electrolyte.
In accordance with similar systems reported elsewhere135,136,137, the transient photocurrent response of the composite may be modelled as a function of time since the onset of illumination, ton, using a bi-exponential relationship of the form
where If,on and Is,on respectively denote the equilibrium contributions of “fast” and “slow” processes, described by the characteristic time constants τf,on and τs,on, respectively, to overall photocurrent I. Similarly, relaxation of the photocurrent following turn-off of the LED source may be described as a function of the time since turn-off, toff, by the formula
where processes such as the generation and recombination of electron-hole pairs in CdS and electron transfer to and from WOx are once again categorised as either “fast” or “slow”, with associated time constants τf,off and τs,off and initial photocurrents If,off and Is,off, respectively. It is to be additionally assumed that each electrode was chemically stable in the absence of light, and therefore any time-dependence of the variables If,off and Is,off in Eq. 2 is to be ignored. Conversely, If,on and Is,on are to be modelled using mono-exponential relationships with respect to ton given by
where the suffix “x” must be substituted for either “f” or “s”, Ax,on is a multiplicative constant that may differ between fast and slow processes, and the constants I0, It and τd are assumed independent of process and time. Recognising that τd is likely to be much larger than τf,on and τs,on, Eq. 1 reduces to a form proportional to Eq. 3 in the limit of large ton; moreover, one may impose the arbitrary condition that Af,on and As,on sum to unity, whereupon I0, It and τd remain as the only free variables within the approximation. In this way, three of the seven free variables in Eq. 1 may be determined prior to its application as a fitting function for transient response measurements close to the onset of illumination.
The decay of photocurrent during prolonged illumination of the CdS and CdS/WOx samples is shown in Fig. 9a,b, respectively, with the form of the diminishing response fitted in the latter case using Eqs 1, 3 for ton values greater than 2,000 s; from this fit, a τd estimate of 4167.3 ± 1.5 s is acquired for the CdS/WOx electrode, alongside I0 and It values of 1.2218 ± (1.7 × 10−3) μA and 14.7356 ± (1.0 × 10−3) μA, respectively. The transient response of the CdS/WOx system has been subsequently modelled using the exact form of Eq. 1, as shown in Fig. 9c; in conjunction with the three estimated variables from Fig. 9b, the depicted curve is well-characterised by respective τf,on and τs,on values of 81.24 ± 0.12 s and 381.5 ± 0.2 s, with Af,on and As,on estimated as 0.3637 ± (5 × 10−4) and 0.6363 ± (5 × 10−4), respectively. Similarly, the relaxation curve in Fig. 9d has been fitted by Eq. 2 using values of 110.9 ± 1.0 s and 547.2 ± 1.0 s for τf,off and τs,off, respectively, in addition to respective values of 0.827 ± (5 × 10−3) μA and 2.077 ± (5 × 10−3) μA for If,off and Is,off.
Having explored the photocapacitive behaviour of the CdS/WOx composite, it is important to compare the characteristics to corresponding measurements from similar materials. Unfortunately, precise comparison with previous CdS/WOx composites is difficult because, to the authors’ knowledge, researchers have yet to explore the photocapacitive properties of this material combination; nevertheless, there exist studies which briefly report the photocurrent response of CdS/WOx composites, albeit without any focus on the self-charging behaviour55,57,105. Relative to these previous examples, the present composite exhibited a superior initial photocurrent response and a similar response after multiple cycles: under similar experimental conditions, other CdS/WOx composites typically yielded photocurrents of around 10 µA cm−2. Additionally, the rate of discharge in the cited works was significantly more rapid than in the present case: as shown by Fig. 9d, a current was measured from the CdS/WOx composite more than twenty minutes after final illumination. In the work by Zhang et al.57, by contrast, near-total discharge was achieved within a period of approximately 20 s, whereas the material synthesised by Jin et al.55 exhibited a discharge time of approximately 60 s. Other binary composites produced similar short-circuit discharge currents, with discharge times of less than 60 s typical for these materials27,28,29,138,139,140. In the majority of the cited examples, including those corresponding to CdS/WOx composites, the discharge current decreased to less than half of its original value almost instantly upon turn-off of the light source, in stark contrast to the comparatively gradual rate of discharge shown in Fig. 9d.
When investigating the behaviour of capacitive systems, a conventional approach is to estimate the specific capacitance of an electrode through cyclic voltammetry or galvanostatic charge/discharge measurements141,142,143,144,145. Though useful, it has been argued elsewhere that these experiments are unfortunately misleading when a system behaves as a current source in addition to its supercapacitive properties146. Moreover, due to the rudimentary drop-casting approach adopted for electrode preparation in the present study, sample inhomogeneity and incomplete adhesion of the sample materials to the underlying FTO-coated glass prohibited meaningful estimation of the specific capacitance. It is for these reasons that the present investigation is focussed on the form of the photoresponse under short-circuit and open-circuit conditions, in addition to addressing the electronic mechanisms responsible for the observed behaviours.
By examining the photocurrent response and open circuit potential of a CdS/WOx composite under white LED illumination, the photocapacitive properties of the material have been demonstrated. At a power density of 99.3 mW cm−2, the sample out-performed existing CdS/WOx composites in photoelectrochemical tests, exhibiting a similar photocurrent response after multiple illumination cycles but a markedly superior ability to store photoinduced charge: short-circuit current persisted for more than twenty minutes after final illumination, compared to less than a minute in previous examples from the literature.
Based on the electronic band edge positions deduced from XPS, UPS and UV-Vis diffuse reflectance measurements, it has been surmised that the measured charge-accumulation in CdS/WOx resulted from the trapping of photoexcited electrons from CdS following their transfer to the conduction band of WOx. Moreover, the enhancement of photocurrent with respect to a CdS control sample may be attributed in part to the quenching of valence holes at the CdS/WOx interface, thereby extending the mean lifetime of photoexcited electrons by suppressing electron-hole recombination within the CdS component. These deductions are supported by similar measurements from a Ta3N5/WOx reference sample, which was synthesised using an analogous solvothermal protocol: the Ta3N5/WOx composite and separate Ta3N5 and WOx reference electrodes produced no significant photocurrent response under LED illumination, indicating that the photocapacitive characteristics of CdS/WOx resulted from a synergistic electronic relationship between its constituents and not from one component in isolation.
With solar technologies likely to play a critical role in future energy production, self-charging materials are a potentially invaluable commodity. In showcasing the photocapacitive behaviour of a CdS/WOx composite, the present study provides a seminal insight into the promise of this material combination. Building on this work, one might conceive of a layered, self-charging solar cell that utilises CdS for the photogeneration of electron-hole pairs and an adjoining WOx layer for subsequent charge storage. Furthermore, since the self-charging performance of the present composite was superior to other CdS/WOx composites reported in the literature, it is likely that further improvement might be achieved through optimisation of the synthesis protocol; it would be instructive, for instance, to explore the effects of varying the relative quantities of the two constituents or, alternatively, the size or shape of the CdS or WOx particles.
Within this seminal investigation into CdS/WOx composites for self-charging solar applications, the viability of the system has been demonstrated in a predominantly qualitative manner. There remains significant scope for development with respect to the uniformity of the working electrode and its mechanical stability. Mitigation of these problems and more quantitative measurement of properties such as the specific capacitance, as well as examination of the factors affecting the chemical stability of the composite, are left to future work; nevertheless, the present study serves as a valuable foundation for additional research.
CdS nanoparticles were grown using a solvothermal technique adapted from the literature147. Cadmium(II) acetate dihydrate (10 mmol) and thiourea (20 mmol) were dissolved in deionised water (60 ml), before the solution was transferred to a PTFE cup of 125 ml capacity which was in turn secured inside a stainless steel Parr acid digestion bomb. The vessel was heated in a muffle furnace to 180 °C at a rate of 10 °C min−1, and was maintained at this temperature for ten hours. After cooling naturally to room temperature, the resulting orange precipitate was cleaned through repeated centrifugation into deionised water and then absolute ethanol, before being dried overnight at 80 °C and subsequently ground into a fine powder using a pestle and mortar.
Synthesis of the CdS/WOx composite was achieved using a second solvothermal step. CdS nanoparticles (20 mM) were added to a solution of tungsten(VI) chloride (20 mM) in 4:1 v/v mixture of absolute ethanol and ethylene glycol. The resulting suspension was transferred to a PTFE cup of 125 ml capacity and secured inside a stainless steel Parr acid digestion bomb. Using a muffle furnace, the suspension was heated at a rate of 10 °C min−1 to 180 °C, and this temperature was held constant for a period of 24 hours. The vessel was subsequently cooled naturally to room temperature, and the dark-green precipitate was obtained by centrifuging repeatedly into deionised water and then absolute ethanol, followed by drying overnight at 80 °C. The dried material was finally ground into a fine powder using a pestle and mortar.
Ta3N5, WOx and Ta3N5/WOx reference samples
To serve as reference samples, nanoparticles of tantalum(V) nitride, Ta3N5, tungsten(VI) sub-oxide, WOx, and a nanocomposite of tantalum(V) nitride and tungsten(VI) sub-oxide, Ta3N5/WOx, were synthesised using procedures described elsewhere59. In brief, the Ta3N5 nanoparticles were prepared inside a tube furnace by annealing a mixture of tantalum(V) chloride (2.0 mmol), sodium chloride (2.8 mmol) and potassium chloride (1.2 mmol) at 800 °C for ten hours under continuous flow of ammonia gas. The Ta3N5/WOx composite was subsequently obtained using a technique analogous to that described for CdS/WOx, with the CdS substituted for Ta3N5 (3.8 mM) and tungsten(VI) chloride present at a slightly increased concentration of 22.8 mM. All other reaction conditions, including the heating parameters, the composition and volume of the solvent, and the centrifugation steps used to clean the final precipitate, remained the same as in the CdS/WOx case. To prepare the WOx reference sample, an ethanolic solution of WCl6 (12.6 mM, 70 ml) was transferred to a 125 ml PTFE cup and heated at a rate of 10 °C min−1 in the 125 ml stainless steel Parr acid digestion bomb to a temperature of 180 °C, which was maintained for 24 hours. The resulting flocculent blue precipitate was centrifuged into ethanol and then deionised water, before drying overnight at a temperature of 80 °C. All reference materials were ground into a fine powder using a pestle and mortar.
SEM and EDX characterization
For SEM analysis, powders of CdS and CdS/WOx were deposited onto separate adhesive carbon tabs and examined using a Hitachi S4800 FE-SEM, with the accelerating voltage set to 10 kV and an emission current of 10 µA. Within the analysis chamber of the FE-SEM instrument, the elemental composition of each sample was measured at 5,000-times magnification using an Oxford Instruments Silicon Drift X-Max energy-dispersive X-ray (EDX) detector with 50 mm2 active area; the spectrum was recorded at an accelerating voltage of 20 kV and an emission current of 10 µA, and was subsequently analysed using Oxford Instruments INCA EDX software.
The crystal structures of CdS and CdS/WOx were investigated through X-ray diffractometry carried out using a Bruker D8 Advance X-ray diffractometer. For these measurements, a small quantity of each material was transferred into a special glass capillary of 0.5 mm diameter, and the diffractograms were acquired using Cu-Kα radiation in conjunction with a Ni filter. The step-size employed was 0.015°, with an acquisition time of 10 s per step and a 2θ range of 10° to 90°.
UV-Vis diffuse reflectance measurements were carried out for samples of CdS and CdS/WOx by transferring each powder to a spring-loaded powder cell in an Agilent Cary 100 UV-Vis spectrophotometer, with the spectra referenced to a Labsphere Spectralon diffuse reflectance standard. The spectra were recorded using a quartz-iodide lamp over a wavelength range of 400–800 nm, with a step size of 1 nm and 100 ms per step. From the diffuse reflectance spectra, Tauc plots were constructed using a Matlab program, which also provided an estimate of the band-gap by extrapolating a line-of-best-fit through the point of steepest gradient on the absorption cut-off curve.
XPS and UPS measurements
The surface chemical composition of each sample was investigated through XPS analysis. Spectra were recorded using a Kratos Axis Supra system employing a monochromated Al-Kα X-ray source; for these measurements, the CdS and CdS/WOx powders were each compressed using a two-tonne press into a circular pellet of 5 mm diameter and mounted on conductive copper tape. To maximise electrical contact between the sample plate and the pellet surface, copper clips were screwed in place over a portion of each pellet, leaving the remainder exposed for measurement. Survey spectra were recorded across binding energies of 0–1200 eV using pass energy 160 eV, dwell time 100 ms and step size 1 eV. With the exceptions of the Cd 3d peak of CdS and the W 4f, O 1 s and Cd 3d peaks of CdS/WOx, core level peaks of interest were measured using pass energy 20 eV, dwell time 1500 ms and step size 50 meV, and averaging over three sweeps; in the case of the other core level peaks of interest, the same pass energy, step size and number of repeat scans were used, but the dwell time was reduced to a value of 500 ms for the Cd 3d peak of CdS and a dwell time of 1000 ms was employed for the W 4f, O 1 s and Cd 3d peaks of CdS/WOx. All XPS measurements were performed over a rectangular area of 700 × 300 µm.
Surface charge compensation during the XPS measurements was achieved using a charge neutraliser operating at a charge balance potential of 3.3 V, filament bias 1.0 V and filament current 0.4 A. The spectra were “carbon-corrected”, with the binding energy scale shifted by the value required to reference the C 1 s peak to 284.8 eV, the accepted value for the predominant sp3 carbon environments of adventitious organic contaminants89. Each core level peak was deconvoluted using Gaussian-Lorentzian product functions, while the contribution of the secondary electron background was modelled using a Shirley-type function. In the case of a doublet, the relative areas of the two components were constrained following consideration of spin population statistics, and the requisite spin-orbit splitting was imposed accordingly. With the exception of the W 4f signal of CdS/WOx, the full widths at half maximum of components within a particular peak were constrained to be equal; conversely, it was ensured that 4f5/2 and 4f7/2 components associated with a particular chemical environment of the W 4f peak were set equal, but components corresponding to different environments were allowed different peak widths. Moreover, while most of the peak fitting was achieved using Gaussian-Lorentzian product functions with 30% Lorentzian character, those of the W 4f signal possessed 80% Lorentzian character due to the greater asymmetry required for the fit. Atomic ratios of different elements were calculated by dividing the areas of the fitted components by the relevant relative sensitivity factors.
To determine the valence band maximum position of each sample, XPS measurements were performed at binding energies close to the Fermi edge position at 0 eV. These scans were undertaken using pass energy 20 eV, dwell time 1500 ms and step size 50 meV, averaging over three sweeps. The ionisation potential of each sample was estimated through use of UPS; to prepare the pelletised samples for these measurements, surface contamination was first removed by bombarding a 4 × 4 mm area with 1000+ atom argon ion clusters of total energy 10 keV for a period of 120 s. Measurements were subsequently carried out using a He I source (21.22 eV photon energy) over a kinetic energy range of 0.4–23.0 eV, using pass energy 5 eV, step size 25 meV, 60 ms dwell time and a 55 µm diameter aperture, followed by an additional scan in each case between kinetic energies of 8.0 eV and 23.0 eV, with the same pass energy, step size and dwell time but an aperture of diameter 110 µm. All UPS measurements employed a −9 V sample bias potential.
For measurements of the electrical response to white light illumination under both short-circuit and open-circuit conditions, electrodes were prepared using fluorine-doped tin oxide (FTO)-coated glass with a sheet resistance of 7 Ω per square. Prior to fabrication, the FTO-coated glass was cut into a 50 × 25 mm rectangle and cleaned thoroughly by ultra-sonication in acetone followed by isopropanol. After masking a 15 × 15 mm square area with scotch tape and providing electrical contact to the top of the electrode via a copper wire secured with copper tape, the remainder of the electrode was electrically isolated using a UV-cured glass-fibre epoxy resin. The scotch tape was subsequently removed and the exposed area cleaned once more with acetone and isopropanol. To deposit the sample material, sample powder (10 mg) was first suspended in absolute ethanol (1 ml), with ultra-sonication employed to ensure a homogenous suspension. Maintaining the electrode at a temperature of 70 °C on a hot-plate, the material was sequentially layered onto the exposed area through stepwise drop-casting of the suspension, allowing the material to dry completely between successive steps.
White light illumination was provided by a custom-built light box containing a 40 W LED source, which provided a radiant flux density of 99.3 ± 0.6 mW cm−2 to the sample. Measurement of the luminous flux density was carried out using an Extech EA33 EasyView light meter, while the form of the spectrum was recorded by an Ocean Optics USB 2000+ spectrometer. Estimation of the radiant flux density from these measurements was achieved through use of the CIE standard photopic luminous efficacy function148,149,150,151; further details regarding this calculation and the measured form of the LED spectrum are provided by Fig. S3 of the Supplementary Information and the accompanying discussion.
For all photoelectrochemical measurements, electrodes were immersed in an aqueous solution of Na2SO4 (0.5 M) and the tests were performed using a three-electrode setup with an Ag/AgCl (3.0 M) reference and platinum mesh counter electrode. In each case, the FTO-coated glass working electrode was configured for back-side illumination. Both the reference and counter electrodes were rinsed thoroughly with deionised water between testing of different sample electrodes, and the aqueous Na2SO4 electrolyte was also replaced.
To investigate the transient photocurrent response of the samples, a potential difference of 0 V was applied between the working and reference electrodes and the current passing between the working and counter electrodes was measured during white light illumination. Initial measurements were carried out using chopped LED illumination with a period of approximately 330 s, before the sample electrode was rinsed in deionised water, allowed to dry naturally and left overnight in darkness. The electrode was then reintroduced to the three-electrode setup as before with a fresh batch of electrolyte solution, and exposed to the LED light continuously for several hours to observe the photocurrent variation during prolonged illumination. Photocurrent response and relaxation curves were fitted using a non-linear regression protocol carried out by a Matlab program, with the standard error in each fitting parameter calculated from the square root of the diagonalised covariance matrix generated by the regression function.
After returning the setup to darkness and allowing the photocurrent to diminish to a stable value close to zero, the open-circuit potential of each sample electrode was investigated. With the current between the sample and counter electrodes constrained to zero, the LED remained off until a stable potential difference was attained between the sample and reference electrodes. Once stabilised, the system was illuminated continuously for several hours to observe the variation of the potential difference as a function of exposure time, and the relaxation of the system was subsequently explored after turn-off of the LED source.
Agnew, S. & Dargusch, P. Consumer preferences for household-level battery energy storage. Renew. Sust. Energ. Rev. 75, 609–617 (2017).
Speidel, S. & Bräunl, T. Leaving the grid—The effect of combining home energy storage with renewable energy generation. Renew. Sust. Energ. Rev. 60, 1213–1224 (2016).
Truong, C. et al. Economics of Residential Photovoltaic Battery Systems in Germany: The Case of Tesla’s Powerwall. Batteries 2, 14 (2016).
Zhang, C., Wei, Y.-L., Cao, P.-F. & Lin, M.-C. Energy storage system: Current studies on batteries and power condition system. Renew. Sust. Energ. Rev. 82, 3091–3106 (2018).
Phillips, R. & Dunnill, C. W. Zero Gap Alkaline Electrolysis Cell Designs for Renewable Energy Storage as Hydrogen Gas. RSC Adv. 6, 100643 (2016).
Phillips, R., Edwards, A., Rome, B., Jones, D. R. & Dunnill, C. W. Minimising the ohmic resistance of an alkaline electrolysis cell through effective cell design. Int. J. Hydrogen Energ. 42, 23986–23994 (2017).
Passas, G. & Dunnill, C. W. Water Splitting Test Cell for Renewable Energy Storage as Hydrogen Gas. J. Fundam. Renewable Energy Appl. 5, 188 (2015).
Paul, B. & Andrews, J. PEM unitised reversible/regenerative hydrogen fuel cell systems: State of the art and technical challenges. Renew. Sust. Energ. Rev. 79, 585–599 (2017).
Eriksson, E. L. V. & Gray, E. M. Optimization and integration of hybrid renewable energy hydrogen fuel cell energy systems – A critical review. Appl. Energ. 202, 348–364 (2017).
Jones, D. R., Al-Masry, W. A. & Dunnill, C. W. Hydrogen-enriched natural gas as a domestic fuel: an analysis based on flash-back and blow-off limits for domestic natural gas appliances within the UK. Sustainable Energy Fuels 2, 710–723 (2018).
Kapila, S., Oni, A. O. & Kumar, A. The development of techno-economic models for large-scale energy storage systems. Energy 140, 656–672 (2017).
Hoppmann, J., Volland, J., Schmidt, T. S. & Hoffmann, V. H. The economic viability of battery storage for residential solar photovoltaic systems – A review and a simulation model. Renew. Sust. Energ. Rev. 39, 1101–1118 (2014).
Balcombe, P., Rigby, D. & Azapagic, A. Energy self-sufficiency, grid demand variability and consumer costs: Integrating solar PV, Stirling engine CHP and battery storage. Appl. Energ. 155, 393–408 (2015).
Weniger, J., Tjaden, T. & Quaschning, V. Sizing of Residential PV Battery Systems. Energy Procedia 46, 78–87 (2014).
Pu, X., Hu, W. & Wang, Z. L. Toward Wearable Self-Charging Power Systems: The Integration of Energy-Harvesting and Storage Devices. Small 14, 1702817 (2018).
Baek, S.-W. et al. A Colloidal-Quantum-Dot-Based Self-Charging System via the Near-Infrared Band. Adv. Mater., 1707224 (2018).
Liu, H., Li, M., Kaner, R. B., Chen, S. & Pei, Q. Monolithically Integrated Self-Charging Power Pack Consisting of a Silicon Nanowire Array/Conductive Polymer Hybrid Solar Cell and a Laser-Scribed Graphene Supercapacitor. ACS Appl. Mater. Interfaces 10, 15609–15615 (2018).
Liu, R. et al. Silicon Nanowire/Polymer Hybrid Solar Cell-Supercapacitor: A Self-Charging Power Unit with a Total Efficiency of 10.5%. Nano Lett. 17, 4240–4247 (2017).
Zhang, Z. et al. Integrated Polymer Solar Cell and Electrochemical Supercapacitor in a Flexible and Stable Fiber Format. Adv. Mater. 26, 466–470 (2014).
Sandbaumhüter, F. et al. Compatibility study towards monolithic self-charging power unit based on all-solid thin-film solar module and battery. J. Power Sources 365, 303–307 (2017).
van Leeuwen, N. S. et al. Residual Energy Harvesting from Light Transients Using Hematite as an Intrinsic Photocapacitor in a Symmetrical Cell. ACS Appl. Energy Mater. 1, 38–42 (2017).
Liu, R., Liu, C. & Fan, S. A photocapacitor based on organometal halide perovskite and PANI/CNT composites integrated using a CNT bridge. J. Mater. Chem. A 5, 23078–23084 (2017).
Liu, Z. et al. Novel Integration of Perovskite Solar Cell and Supercapacitor Based on Carbon Electrode for Hybridizing Energy Conversion and Storage. ACS Appl. Mater. Interfaces 9, 22361–22368 (2017).
Miyasaka, T. & Murakami, T. N. The photocapacitor: An efficient self-charging capacitor for direct storage of solar energy. Appl. Phys. Lett. 85, 3932–3934 (2004).
Safshekan, S. et al. Solar Energy Storage by a Heterostructured BiVO4–PbOx Photocapacitive Device. ACS Energy Lett. 2, 469–475 (2017).
Agiorgousis, M. L., Sun, Y.-Y., West, D. & Zhang, S. Intercalated Chevrel Phase Mo6S8 as a Janus Material for Energy Generation and Storage. ACS Appl. Energy Mater. 1, 440–446 (2018).
Prabhu, S., Manikumar, S., Cindrella, L. & Kwon, O. J. Charge transfer and intrinsic electronic properties of rGO-WO3 nanostructures for efficient photoelectrochemical and photocatalytic applications. Mater. Sci. Semicond. Process. 74, 136–146 (2018).
Usui, H., Suzuki, S., Domi, Y. & Sakaguchi, H. TiO2/MnO2 composite electrode enabling photoelectric conversion and energy storage as photoelectrochemical capacitor. Mater. Today Energy 9, 229–234 (2018).
Narayanan, R., Kumar, P. N., Deepa, M. & Srivastava, A. K. Combining Energy Conversion and Storage: A Solar Powered Supercapacitor. Electrochim. Acta 178, 113–126 (2015).
Su, Y., Ao, D., Liu, H. & Wang, Y. MOF-derived yolk–shell CdS microcubes with enhanced visible-light photocatalytic activity and stability for hydrogen evolution. J. Mater. Chem. A 5, 8680–8689 (2017).
Ning, X., Meng, S., Fu, X., Ye, X. & Chen, S. Efficient utilization of photogenerated electrons and holes for photocatalytic selective organic syntheses in one reaction system using a narrow band gap CdS photocatalyst. Green Chem. 18, 3628–3639 (2016).
Lisco, F. et al. The structural properties of CdS deposited by chemical bath deposition and pulsed direct current magnetron sputtering. Thin Solid Films 582, 323–327 (2015).
Zhang, L. et al. Ultra-low content of Pt modified CdS nanorods: one-pot synthesis and high photocatalytic activity for H2 production under visible light. J. Mater. Chem. A 3, 23732–23742 (2015).
Guo, Y. et al. RF sputtered CdS films as independent or buffered electron transport layer for efficient planar perovskite solar cell. Sol. Energ. Mat. Sol. C. 178, 186–192 (2018).
Abulikemu, M., Barbé, J., El Labban, A., Eid, J. & Del Gobbo, S. Planar heterojunction perovskite solar cell based on CdS electron transport layer. Thin Solid Films 636, 512–518 (2017).
Powell, M. J., Dunnill, C. W. & Parkin, I. P. N-doped TiO2 visible light photocatalyst films via a sol–gel route using TMEDA as the nitrogen source. J. Photoch. Photobiol. A 281, 27–34 (2014).
Dunnill, C. W. H. et al. Enhanced photocatalytic activity under visible light in N-doped TiO2 thin films produced by APCVD preparations using t-butylamine as a nitrogen source and their potential for antibacterial films. J. Photoch. Photobiol. A 207, 244–253 (2009).
Warwick, M. E. A., Dunnill, C. W. & Binions, R. Multifunctional Nanocomposite Thin Films by Aerosol-Assisted CVD. Chem. Vap. Depos. 16, 220–224 (2010).
Tang, Y., Hu, X. & Liu, C. Perfect inhibition of CdS photocorrosion by graphene sheltering engineering on TiO2 nanotube array for highly stable photocatalytic activity. Phys. Chem. Chem. Phys. 16, 25321–25329 (2014).
Yang, M.-Q., Han, C. & Xu, Y.-J. Insight into the Effect of Highly Dispersed MoS2 versus Layer-Structured MoS2 on the Photocorrosion and Photoactivity of CdS in Graphene–CdS–MoS2 Composites. J. Phys. Chem. C 119, 27234–27246 (2015).
Villa, K., Domènech, X., García-Pérez, U. M. & Peral, J. Photocatalytic Hydrogen Production Under Visible Light by Using a CdS/WO3 Composite. Catal. Lett. 146, 100–108 (2015).
Fermin, D. J., Ponomarev, E. A. & Peter, L. M. A kinetic study of CdS photocorrosion by intensity modulated photocurrent and photoelectrochemical impedance spectroscopy. J. Electroanal. Chem. 473, 192–203 (1999).
Chen, S. & Wang, L.-W. Thermodynamic Oxidation and Reduction Potentials of Photocatalytic Semiconductors in Aqueous Solution. Chem. Mater. 24, 3659–3666 (2012).
Meissner, D., Memming, R. & Kastening, B. Photoelectrochemistry of Cadmium Sulfide. 1. Reanalysis of Photocorrosion and Flat-Band Potential. J. Phys. Chem. 92, 3476–3483 (1988).
Zheng, H. et al. Nanostructured Tungsten Oxide - Properties, Synthesis, and Applications. Adv. Funct. Mater. 21, 2175–2196 (2011).
Cong, S. et al. Noble metal-comparable SERS enhancement from semiconducting metal oxides by making oxygen vacancies. Nat. Commun. 6, 7800 (2015).
Zhou, H. et al. Surface Oxygen Vacancy-Dependent Electrocatalytic Activity of W18O49 Nanowires. J. Phys. Chem. C 118, 20100–20106 (2014).
Epifani, M. et al. Solvothermal, Chloroalkoxide-based Synthesis of Monoclinic WO3 Quantum Dots and Gas-Sensing Enhancement by Surface Oxygen Vacancies. ACS Appl. Mater. Interfaces 6, 16808–16816 (2014).
Dunnill, C. W., Noimark, S. & Parkin, I. P. Silver loaded WO3-x/TiO2 composite multifunctional thin films. Thin Solid Films 520, 5516–5520 (2012).
Wang, G., Ling, Y. & Li, Y. Oxygen-deficient metal oxide nanostructures for photoelectrochemical water oxidation and other applications. Nanoscale 4, 6682 (2012).
Wang, Q., Puntambekar, A. & Chakrapani, V. Vacancy-Induced Semiconductor–Insulator–Metal Transitions in Nonstoichiometric Nickel and Tungsten Oxides. Nano Lett. 16, 7067–7077 (2016).
Vasilopoulou, M. et al. Influence of the Oxygen Substoichiometry and of the Hydrogen Incorporation on the Electronic Band Structure of Amorphous Tungsten Oxide Films. J. Phys. Chem. C 118, 12632–12641 (2014).
Shifu, C., Lei, C., Shen, G. & Gengyu, C. The preparation of coupled WO3/TiO2 photocatalyst by ball milling. Powder Technol. 160, 198–202 (2005).
Sotelo-Vazquez, C. et al. Evidence and Effect of Photogenerated Charge Transfer for Enhanced Photocatalysis in WO3/TiO2 Heterojunction Films: A Computational and Experimental Study. Adv. Funct. Mater. 27, 1605413 (2017).
Jin, J., Yu, J., Guo, D., Cui, C. & Ho, W. A Hierarchical Z-Scheme CdS-WO3 Photocatalyst with Enhanced CO2 Reduction Activity. Small 11, 5262–5271 (2015).
Park, H., Kim, H.-i., Moon, G.-h. & Choi, W. Photoinduced charge transfer processes in solar photocatalysis based on modified TiO2. Energy Environ. Sci. 9, 411–433 (2016).
Zhang, J., Guo, Y., Xiong, Y., Zhou, D. & Dong, S. An environmentally friendly Z-scheme WO3/CDots/CdS heterostructure with remarkable photocatalytic activity and anti-photocorrosion performance. J. Catal. 356, 1–13 (2017).
Rodríguez-Pérez, M., Chacón, C., Palacios-González, E., Rodríguez-Gattorno, G. & Oskam, G. Photoelectrochemical water oxidation at electrophoretically deposited WO3 films as a function of crystal structure and morphology. Electrochim. Acta 140, 320–331 (2014).
Jones, D. R. et al. Active removal of waste dye pollutants using Ta3N5/W18O49 nanocomposite fibres. Sci. Rep. 7, 4090 (2017).
Huang, Z.-F. et al. Synergetic promotion on photoactivity and stability of W18O49/TiO2 hybrid. Appl. Catal. B: Environ. 147, 167–174 (2014).
Chang, X., Dong, L., Yin, Y. & Sun, S. A novel composite photocatalyst based on in situ growth of ultrathin tungsten oxide nanowires on graphene oxide sheets. RSC Adv. 3, 15005 (2013).
Song, K. et al. W18O49 nanowires grown on g-C3N4 sheets with enhanced photocatalytic hydrogen evolution activity under visible light. J. Mol. Catal. A: Chem. 418–419, 95–102 (2016).
Ma, L. et al. Facile method to prepare CdS nanostructure based on the CdTe films. Appl. Surf. Sci. 349, 740–745 (2015).
Zhu, Y., Wang, L., Lai, Y., Chi, L. & Li, Z. Thin films composed of irregular micro-block arrays of closely packed CdS nanoparticles for enhanced photoelectrochemical performance. Electrochem. Commun. 83, 16–19 (2017).
Ehsan, M. A. et al. Effect of AACVD Processing Parameters on the Growth of Greenockite (CdS) Thin Films using a Single-Source Cadmium Precursor. Chem. Vap. Depos. 18, 191–200 (2012).
Roy, P. & Srivastava, S. K. A new approach towards the growth of cadmium sulphide thin film by CBD method and its characterization. Mater. Chem. Phys. 95, 235–241 (2006).
García-Valenzuela, J. A., Nájera-Luna, A. L., Castillo-Ortega, M. M., Hu, H. & Sotelo-Lerma, M. An inexpensive, rapid, safe, and recycling-favoring method for the fabrication of core/shell PVP/CdS composite fibers from a gas–solid reaction between H2S vapor and electrospun PVP/CdCl2. Mater. Sci. Semicond. Process. 38, 257–265 (2015).
Muruganandam, S., Anbalagan, G. & Murugadoss, G. Structural, electrochemical and magnetic properties of codoped (Cu, Mn) CdS nanoparticles with surfactant PVP. Optik 131, 826–837 (2017).
Li, K. et al. Hexagonal@Cubic CdS Core@Shell Nanorod Photocatalyst for Highly Active Production of H2with Unprecedented Stability. Adv. Mater. 28, 8906–8911 (2016).
Slonopas, A. et al. Growth mechanisms and their effects on the opto-electrical properties of CdS thin films prepared by chemical bath deposition. Mater. Sci. Semicond. Process. 52, 24–31 (2016).
Nasalevich, M. A., Kozlova, E. A., Lyubina, T. P. & Vorontsov, A. V. Photocatalytic oxidation of ethanol and isopropanol vapors on cadmium sulfide. J. Catal. 287, 138–148 (2012).
Yue, L. et al. Enhanced reversible lithium storage in ultrathin W18O49 nanowires entwined Si composite anode. Mater. Lett. 187, 118–122 (2017).
Fang, Z., Jiao, S., Kang, Y., Pang, G. & Feng, S. Photothermal Conversion of W18O49 with a Tunable Oxidation State. ChemistryOpen 6, 261–265 (2017).
Zhao, Y., Tang, Q., He, B. & Yang, P. Mo incorporated W18O49 nanofibers as robust electrocatalysts for high-efficiency hydrogen evolution. Int. J. Hydrogen Energ. 42, 14534–14546 (2017).
Welberry, T. R. & Weber, T. One hundred years of diffuse scattering. Crystallogr. Rev. 22, 2–78 (2015).
Khallaf, H. et al. Characterization of gallium-doped CdS thin films grown by chemical bath deposition. Appl. Surf. Sci. 255, 4129–4134 (2009).
Rajeswari Yogamalar, N., Sadhanandham, K., Chandra Bose, A. & Jayavel, R. Band alignment and depletion zone at ZnO/CdS and ZnO/CdSe hetero-structures for temperature independent ammonia vapor sensing. Phys. Chem. Chem. Phys. 18, 32057–32071 (2016).
Zhu, Y. et al. Visible light induced photocatalysis on CdS quantum dots decorated TiO2 nanotube arrays. Appl. Catal. A: Gen. 498, 159–166 (2015).
Tao, J. et al. 7.1% efficient co-electroplated Cu2ZnSnS4 thin film solar cells with sputtered CdS buffer layers. Green Chem. 18, 550–557 (2016).
Weinhardt, L. et al. CdS and Cd(OH)2 formation during Cd treatments of Cu(In,Ga)(S,Se)2 thin-film solar cell absorbers. Appl. Phys. Lett. 82, 571–573 (2003).
Bär, M. et al. CdS/Low-Band-Gap Kesterite Thin-Film Solar Cell Absorber Heterojunction: Energy Level Alignment and Dominant Recombination Process. ACS Appl. Energy Mater. 1, 475–482 (2018).
Mazón-Montijo, D. A., Sotelo-Lerma, M., Rodríguez-Fernández, L. & Huerta, L. AFM, XPS and RBS studies of the growth process of CdS thin films on ITO/glass substrates deposited using an ammonia-free chemical process. Appl. Surf. Sci. 256, 4280–4287 (2010).
Li, Y., Gao, D., Peng, S., Lu, G. & Li, S. Photocatalytic hydrogen evolution over Pt/Cd0.5Zn0.5S from saltwater using glucose as electron donor: An investigation of the influence of electrolyte NaCl. Int. J. Hydrogen Energ. 36, 4291–4297 (2011).
Yao, P.-C. & Chen, C.-Y. Effect of protic solvents on CdS thin films prepared by chemical bath deposition. Thin Solid Films 579, 103–109 (2015).
El Maliki, H. et al. Study of the influence of annealing on the properties of CBD-CdS thin films. Appl. Surf. Sci. 205, 65–79 (2003).
Maticiuc, N., Katerski, A., Danilson, M., Krunks, M. & Hiie, J. XPS study of OH impurity in solution processed CdS thin films. Sol. Energ. Mat. Sol. C. 160, 211–216 (2017).
Jin, Z., Li, Q., Xi, C., Jian, Z. & Chen, Z. Effect of high-temperature treatment in air ambience on the surface compositions and structure of CdS. Appl. Surf. Sci. 32, 218–232 (1988).
Jiang, X. et al. Effects of molecular interface modification in CdS/polymer hybrid bulk heterojunction solar cells. Sol. Energ. Mat. Sol. C. 94, 2223–2229 (2010).
McCafferty, E. & Wightman, J. P. Determination of the Concentration of Surface Hydroxyl Groups on Metal Oxide Films by a Quantitative XPS Method. Surf. Interface Anal. 26, 549–564 (1998).
Saleem, M. et al. Influence of hydrogen annealing on the optoelectronic properties of WO3 thin films. Int. J. Hydrogen Energ. 40, 12343–12351 (2015).
Bertus, L. M. et al. Synthesis and characterization of WO3 thin films by surfactant assisted spray pyrolysis for electrochromic applications. Mater. Chem. Phys. 140, 49–59 (2013).
Ghasempour, F., Azimirad, R., Amini, A. & Akhavan, O. Visible light photoinactivation of bacteria by tungsten oxide nanostructures formed on a tungsten foil. Appl. Surf. Sci. 338, 55–60 (2015).
Zhang, N. et al. Defective Tungsten Oxide Hydrate Nanosheets for Boosting Aerobic Coupling of Amines: Synergistic Catalysis by Oxygen Vacancies and Brønsted Acid Sites. Small 13, 1701354 (2017).
Wang, R. et al. Enhanced visible-light-driven photocatalytic sterilization of tungsten trioxide by surface-engineering oxygen vacancy and carbon matrix. Chem. Eng. J. 348, 292–300 (2018).
Hai, G. et al. Influence of oxygen deficiency on the synthesis of tungsten oxide and the photocatalytic activity for the removal of organic dye. J. Alloys Compd. 690, 239–248 (2017).
Li, S., Yao, Z., Zhou, J., Zhang, R. & Shen, H. Fabrication and characterization of WO3 thin films on silicon surface by thermal evaporation. Mater. Lett. 195, 213–216 (2017).
Linsmeier, C. et al. Binary beryllium–tungsten mixed materials. J. Nucl. Mater. 363–365, 1129–1137 (2007).
Peng, R. et al. Insight into band positions and inter-particle electron transfer dynamics between CdS nanoclusters and spatially isolated TiO2 dispersed in cubic MCM-48 mesoporous materials: a highly efficient system for photocatalytic hydrogen evolution under visible light illumination. Phys. Chem. Chem. Phys. 16, 2048–2061 (2014).
Khan, M. M. et al. Band gap engineered TiO2 nanoparticles for visible light induced photoelectrochemical and photocatalytic studies. J. Mater. Chem. A 2, 637–644 (2014).
Lv, Y., Yao, W., Zong, R. & Zhu, Y. Fabrication of Wide–Range–Visible Photocatalyst Bi2WO6−x nanoplates via Surface Oxygen Vacancies. Sci. Rep. 6, 19347 (2016).
Bai, S. et al. Boosting Photocatalytic Water Splitting: Interfacial Charge Polarization in Atomically Controlled Core-Shell Cocatalysts. Angew. Chem. Int. Ed. 54, 14810–14814 (2015).
Hashimoto, S. & Matsuoka, H. Mechanism of electrochromism for amorphous WO3 thin films. J. Appl. Phys. 69, 933 (1991).
Solonin, Y. M., Khyzhun, O. Y. & Graivoronskaya, E. A. Nonstoichiometric Tungsten Oxide Based on Hexagonal WO3. Cryst. Growth Des. 1, 473–477 (2001).
Migas, D. B., Shaposhnikov, V. L. & Borisenko, V. E. Tungsten oxides. II. The metallic nature of Magnéli phases. J. Appl. Phys. 108, 093714 (2010).
Kim, H.-i., Kim, J., Kim, W. & Choi, W. Enhanced Photocatalytic and Photoelectrochemical Activity in the Ternary Hybrid of CdS/TiO2/WO3 through the Cascadal Electron Transfer. J. Phys. Chem. C 115, 9797–9805 (2011).
Liu, X. et al. Synergy of adsorption and visible-light photocatalytic degradation of methylene blue by a bifunctional Z-scheme heterojunction of WO 3 /g-C3 N4. Appl. Surf. Sci. 405, 359–371 (2017).
Tersoff, J. Schottky barriers and semiconductor band structures. Phys. Rev. B 32, 6968–6971 (1985).
Tung, R. T. Chemical Bonding and Fermi Level Pinning at Metal-Semiconductor Interfaces. Phys. Rev. Lett. 84, 6078–6081 (2000).
Bard, A. J., Bocarsly, A. B., Fan, F.-R. F., Walton, E. G. & Wrighton, M. S. The Concept of Fermi Level Pinning at Semiconductor/Liquid Junctions. Consequences for Energy Conversion Efficiency and Selection of Useful Solution Redox Couples in Solar Devices. J. Am. Chem. Soc. 102, 3671–3677 (1980).
Rangel, C. M., Silva, T. M. & Belo, M. D. C. Semiconductor electrochemistry approach to passivity and stress corrosion cracking susceptibility of stainless steels. Electrochim. Acta 50, 5076–5082 (2005).
Aruchamy, A. & Wrighton, M. S. A Comparison of the Interface Energetics for n-Type Cadmium Sulfide/ and Cadmium Telluride/Nonaqueous Electrolyte Junctions. J. Phys. Chem. 84, 2848–2854 (1980).
Roy, A. M., De, G. C., Sasmal, N. & Bhattacharyya, S. S. Determination of the flatband potential of semiconductor particles in suspension by photovoltage measurement. Int. J. Hydrogen Energ. 20, 627–630 (1995).
Ginley, D. S. & Butler, M. A. Flatband Potential of Cadmium Sulfide (CdS) Photoanodes and Its Dependence on Surface Ion Effects. J. Electrochem. Soc. 125, 1968–1974 (1978).
Finlayson, M. F. et al. Determination of Flat-Band Position of CdS Crystals, Films, and Powders by Photocurrent and Impedance Techniques. Photoredox Reaction Mediated by Intragap States. J. Phys. Chem. 89, 5676–5681 (1985).
Stojadinović, S., Tadić, N., Radić, N., Grbić, B. & Vasilić, R. CdS particles modified TiO2 coatings formed by plasma electrolytic oxidation with enhanced photocatalytic activity. Surf. Coat. Technol. 344, 528–533 (2018).
Liang, Y.-C. & Lung, T.-W. Growth of Hydrothermally Derived CdS-Based Nanostructures with Various Crystal Features and Photoactivated Properties. Nanoscale Res. Lett. 11 (2016).
Ijaz, S., Ehsan, M. F., Ashiq, M. N., Karamat, N. & He, T. Preparation of CdS@CeO2 core/shell composite for photocatalytic reduction of CO2 under visible-light irradiation. Appl. Surf. Sci. 390, 550–559 (2016).
Liu, X.-W., Li, W.-W. & Yu, H.-Q. Cathodic catalysts in bioelectrochemical systems for energy recovery from wastewater. Chem. Soc. Rev. 43, 7718–7745 (2014).
Mandati, S., Sarada, B. V., Dey, S. R. & Joshi, S. V. Enhanced photoresponse of Cu(In,Ga)Se2/CdS heterojunction fabricated using economical non-vacuum methods. Electron. Mater. Lett. 11, 618–624 (2015).
Fu, Y. et al. Phase-Modulated Band Alignment in CdS Nanorod/SnSx Nanosheet Hierarchical Heterojunctions toward Efficient Water Splitting. Adv. Funct. Mater. 28, 1706785 (2018).
Ibadurrohman, M. & Hellgardt, K. Photoelectrochemical performance of graphene-modified TiO2 photoanodes in the presence of glycerol as a hole scavenger. Int. J. Hydrogen Energ. 39, 18204–18215 (2014).
Dotan, H., Sivula, K., Grätzel, M., Rothschild, A. & Warren, S. C. Probing the photoelectrochemical properties of hematite (α-Fe2O3) electrodes using hydrogen peroxide as a hole scavenger. Energy Environ. Sci. 4, 958–964 (2011).
Ma, Y., Pendlebury, S. R., Reynal, A., Le Formal, F. & Durrant, J. R. Dynamics of photogenerated holes in undoped BiVO4 photoanodes for solar water oxidation. Chem. Sci. 5, 2964–2973 (2014).
Połczyński, P., Jurczakowski, R. & Grochala, W. Strong and Long-Lived Free-Radical Oxidizer Based on Silver(II). Mechanism of Ag(I) Electrooxidation in Concentrated H2SO4. J. Phys. Chem. C 117, 20689–20696 (2013).
Zhang, C., He, Z., Wu, J. & Fu, D. The Peculiar Roles of Sulfate Electrolytes in BDD Anode Cells. J. Electrochem. Soc. 162, E85–E89 (2015).
Mi, Q., Zhanaidarova, A., Brunschwig, B. S., Gray, H. B. & Lewis, N. S. A quantitative assessment of the competition between water and anion oxidation at WO3 photoanodes in acidic aqueous electrolytes. Energy Environ. Sci. 5, 5694 (2012).
Solarska, R., Santato, C., Jorand-Sartoretti, C., Ulmann, M. & Augustynski, J. Photoelectrolytic oxidation of organic species at mesoporous tungsten trioxide film electrodes under visible light illumination. J. Appl. Electrochem. 35, 715–721 (2005).
Nakajima, T. et al. Sustainable chromic acid oxidation: solar-driven recycling of hexavalent chromium ions for quinone production by WO3 nanosponge photoanodes. J. Mater. Chem. A 6, 110–117 (2018).
Zheng, J. et al. Efficient Degradation of Refractory Organics Using Sulfate Radicals Generated Directly from WO3 Photoelectrode and the Catalytic Reaction of Sulfate. Catalysts 7, 346 (2017).
Ma, M. et al. Dual Oxygen and Tungsten Vacancies on a WO3 Photoanode for Enhanced Water Oxidation. Angew. Chem. Int. Ed. 55, 11819–11823 (2016).
Solarska, R., Jurczakowski, R. & Augustynski, J. A highly stable, efficient visible-light driven water photoelectrolysis system using a nanocrystalline WO3 photoanode and a methane sulfonic acid electrolyte. Nanoscale 4, 1553 (2012).
Zhao, J., Olide, E. & Osterloh, F. E. Enhancing Majority Carrier Transport in WO3 Water Oxidation Photoanode via Electrochemical Doping. J. Electrochem. Soc. 162, H65–H71 (2014).
Huo, N., Yue, Q., Yang, J., Yang, S. & Li, J. Abnormal Photocurrent Response and Enhanced Photocatalytic Activity Induced by Charge Transfer between WS2 Nanosheets and WO3 Nanoparticles. ChemPhysChem 14, 4069–4073 (2013).
Wang, H., Lindgren, T., He, J., Hagfeldt, A. & Lindquist, S.-E. Photolelectrochemistry of Nanostructured WO3 Thin Film Electrodes for Water Oxidation: Mechanism of Electron Transport. J. Phys. Chem. B 104, 5686–5696 (2000).
Guo, D. et al. Zero-Power-Consumption Solar-Blind Photodetector Based on β-Ga2O3/NSTO Heterojunction. ACS Appl. Mater. Interfaces 9, 1619–1628 (2017).
Gheno, A. et al. Printable WO3 electron transporting layer for perovskite solar cells: Influence on device performance and stability. Sol. Energ. Mat. Sol. C. 161, 347–354 (2017).
de Luna Bugallo, A. et al. Visible-blind photodetector based on p–i–n junction GaN nanowire ensembles. Nanotechnology 21, 315201 (2010).
Luo, Q.-P. et al. Reduced Graphene Oxide-Hierarchical ZnO Hollow Sphere Composites with Enhanced Photocurrent and Photocatalytic Activity. J. Phys. Chem. C 116, 8111–8117 (2012).
Huo, P. et al. Incorporation of N–ZnO/CdS/Graphene oxide composite photocatalyst for enhanced photocatalytic activity under visible light. J. Alloys Compd. 670, 198–209 (2016).
Xiang, Q., Yu, J. & Jaroniec, M. Synergetic Effect of MoS2 and Graphene as Cocatalysts for Enhanced Photocatalytic H2 Production Activity of TiO2 Nanoparticles. J. Am. Chem. Soc. 134, 6575–6578 (2012).
Chen, G. Z. Understanding supercapacitors based on nano-hybrid materials with interfacial conjugation. Progress in Natural Science: Materials International 23, 245–255 (2013).
Nwanya, A. C. et al. Electrochromic and electrochemical capacitive properties of tungsten oxide and its polyaniline nanocomposite films obtained by chemical bath deposition method. Electrochim. Acta 128, 218–225 (2014).
Yuksel, R., Durucan, C. & Unalan, H. E. Ternary nanocomposite SWNT/WO3/PANI thin film electrodes for supercapacitors. J. Alloys Compd. 658, 183–189 (2016).
Inamdar, A. I. et al. Highly efficient electro-optically tunable smart-supercapacitors using an oxygen-excess nanograin tungsten oxide thin film. Sol. Energ. Mat. Sol. C. 166, 78–85 (2017).
Fernández, J., Bonastre, J., Molina, J., del Río, A. I. & Cases, F. Study on the specific capacitance of an activated carbon cloth modified with reduced graphene oxide and polyaniline by cyclic voltammetry. Eur. Polym. J. 92, 194–203 (2017).
Akinwolemiwa, B., Peng, C. & Chen, G. Z. Redox Electrolytes in Supercapacitors. J. Electrochem. Soc. 162, A5054–A5059 (2015).
Yu, Z., Yin, B., Qu, F. & Wu, X. Synthesis of self-assembled CdS nanospheres and their photocatalytic activities by photodegradation of organic dye molecules. Chem. Eng. J. 258, 203–209 (2014).
Woods, A. J., Yuen, K. L. & Karvinen, K. S. Characterizing crosstalk in anaglyphic stereoscopic images on LCD monitors and plasma displays. J. Soc. Inf. Disp. 15, 889–898 (2007).
Rea, M. S. The lumen seen in a new light: Making distinctions between light, lighting and neuroscience. Light. Res. Technol. 47, 259–280 (2014).
Blanken, W., Cuaresma, M., Wijffels, R. H. & Janssen, M. Cultivation of microalgae on artificial light comes at a cost. Algal Res. 2, 333–340 (2013).
Cool, S. et al. Development of a High Irradiance LED Configuration for Small Field of View Motion Estimation of Fertilizer Particles. Sensors 15, 28627–28645 (2015).
Financial support was provided by the Welsh Government Sêr Cymru Programme and the Flexis project, which is part-funded by the European Regional Development Fund (ERDF) through the Welsh Government. The authors would like to acknowledge the assistance provided by Swansea University College of Engineering AIM Facility, which was funded in part by the EPSRC (EP/M028267/1), the European Regional Development Fund through the Welsh Government (80708) and the Sêr Solar project via Welsh Government.
The authors declare no competing interests.
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Jones, D.R., Phillips, R., Gannon, W.J.F. et al. Photocapacitive CdS/WOx nanostructures for solar energy storage. Sci Rep 9, 11573 (2019) doi:10.1038/s41598-019-48069-5